#------------------------------------------------------------------------------
#$Date: 2021-05-27 11:33:37 +0300 (Thu, 27 May 2021) $
#$Revision: 265547 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/29/1562918.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562918
loop_
_publ_author_name
'McMillen, Colin D.'
'Emirdag-Eanes, Mehtap'
'Stritzinger, Jared T.'
'Kolis, Joseph W.'
_publ_section_title
;
 Hydrothermal synthesis of new rare earth silicate fluorides: A novel
 class of polar materials
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              155
_journal_page_last               160
_journal_paper_doi               10.1016/j.jssc.2012.02.057
_journal_volume                  195
_journal_year                    2012
_chemical_formula_sum            'F2 Li O8 Si2 Y3'
_chemical_formula_weight         495.85
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 131.13(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   17.651(4)
_cell_length_b                   4.8868(10)
_cell_length_c                   11.625(2)
_cell_measurement_reflns_used    1985
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.7517
_cell_measurement_theta_min      3.0646
_cell_volume                     755.3(4)
_computing_cell_refinement       'CrystalClear (Rigaku/MSC, 1999)'
_computing_data_collection       'CrystalClear (Rigaku/MSC, 1999)'
_computing_data_reduction        'CrystalClear (Rigaku/MSC, 1999)'
_computing_molecular_graphics    'SHELXTL (Bruker-AXS, 1999)'
_computing_publication_material  'SHELXTL (Bruker-AXS, 1999)'
_computing_structure_refinement  'SHELXTL (Bruker-AXS, 1999)'
_computing_structure_solution    'SHELXTL (Bruker-AXS, 1999)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 14.6199
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Rigaku AFC8S'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0819
_diffrn_reflns_av_sigmaI/netI    0.0481
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            3045
_diffrn_reflns_theta_full        25.02
_diffrn_reflns_theta_max         25.02
_diffrn_reflns_theta_min         3.06
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    23.243
_exptl_absorpt_correction_T_max  0.5423
_exptl_absorpt_correction_T_min  0.1185
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'REQAB, CrystalClear'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.361
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'diamond plate'
_exptl_crystal_F_000             920
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.831
_refine_diff_density_min         -1.575
_refine_diff_density_rms         0.301
_refine_ls_extinction_coef       0.0018(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.121
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     76
_refine_ls_number_reflns         658
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.121
_refine_ls_R_factor_all          0.0446
_refine_ls_R_factor_gt           0.0407
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0705P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1067
_refine_ls_wR_factor_ref         0.1105
_reflns_number_gt                597
_reflns_number_total             658
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2012-195-155.cif
_cod_data_source_block           r12
_cod_original_cell_volume        755.2(3)
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               1562918
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Y1 Y 0.0000 -0.21337(19) 0.2500 0.0082(4) Uani 1 2 d S . .
Y2 Y 0.12348(6) -0.20306(13) 0.09154(8) 0.0090(4) Uani 1 1 d . . .
Si1 Si 0.14007(17) 0.2267(4) 0.2939(2) 0.0100(5) Uani 1 1 d . . .
F1 F 0.0757(4) -0.3905(9) 0.4786(5) 0.0185(11) Uani 1 1 d . . .
O1 O 0.1311(4) 0.5581(10) 0.2846(5) 0.0109(12) Uani 1 1 d . . .
O2 O 0.0350(4) 0.0858(9) 0.1386(6) 0.0083(11) Uani 1 1 d . . .
O3 O 0.2246(4) 0.1045(9) 0.2906(6) 0.0113(11) Uani 1 1 d . . .
O4 O 0.1488(4) 0.0809(10) 0.4288(5) 0.0125(11) Uani 1 1 d . . .
Li1 Li 0.2500 0.2500 0.0000 0.035(6) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
F1 Y1 F1 134.1(2) 2 .
F1 Y1 O2 138.75(18) 2 2
F1 Y1 O2 75.27(16) . 2
F1 Y1 O2 75.27(16) 2 .
F1 Y1 O2 138.75(18) . .
O2 Y1 O2 100.7(2) 2 .
F1 Y1 O1 76.68(17) 2 1_545
F1 Y1 O1 81.98(17) . 1_545
O2 Y1 O1 143.77(18) 2 1_545
O2 Y1 O1 78.39(17) . 1_545
F1 Y1 O1 81.98(17) 2 2_545
F1 Y1 O1 76.68(17) . 2_545
O2 Y1 O1 78.39(17) 2 2_545
O2 Y1 O1 143.77(18) . 2_545
O1 Y1 O1 123.4(2) 1_545 2_545
F1 Y1 O4 134.72(16) 2 .
F1 Y1 O4 75.53(17) . .
O2 Y1 O4 71.72(18) 2 .
O2 Y1 O4 64.61(17) . .
O1 Y1 O4 75.55(17) 1_545 .
O1 Y1 O4 143.30(16) 2_545 .
F1 Y1 O4 75.53(17) 2 2
F1 Y1 O4 134.72(16) . 2
O2 Y1 O4 64.61(17) 2 2
O2 Y1 O4 71.72(18) . 2
O1 Y1 O4 143.30(16) 1_545 2
O1 Y1 O4 75.55(17) 2_545 2
O4 Y1 O4 108.8(2) . 2
F1 Y1 Si1 104.96(12) 2 .
F1 Y1 Si1 106.90(13) . .
O2 Y1 Si1 86.91(13) 2 .
O2 Y1 Si1 32.42(14) . .
O1 Y1 Si1 73.07(12) 1_545 .
O1 Y1 Si1 163.53(13) 2_545 .
O4 Y1 Si1 32.24(11) . .
O4 Y1 Si1 91.53(13) 2 .
F1 Y1 Si1 106.90(13) 2 2
F1 Y1 Si1 104.96(12) . 2
O2 Y1 Si1 32.42(14) 2 2
O2 Y1 Si1 86.91(13) . 2
O1 Y1 Si1 163.53(13) 1_545 2
O1 Y1 Si1 73.07(12) 2_545 2
O4 Y1 Si1 91.53(13) . 2
O4 Y1 Si1 32.24(11) 2 2
Si1 Y1 Si1 90.54(8) . 2
F1 Y1 Li1 61.66(13) 2 3_445
F1 Y1 Li1 115.64(13) . 3_445
O2 Y1 Li1 80.33(14) 2 3_445
O2 Y1 Li1 103.68(14) . 3_445
O1 Y1 Li1 135.52(12) 1_545 3_445
O1 Y1 Li1 40.14(12) 2_545 3_445
O4 Y1 Li1 146.21(12) . 3_445
O4 Y1 Li1 39.78(12) 2 3_445
Si1 Y1 Li1 130.24(5) . 3_445
Si1 Y1 Li1 55.23(4) 2 3_445
F1 Y1 Li1 115.64(13) 2 4_545
F1 Y1 Li1 61.66(13) . 4_545
O2 Y1 Li1 103.68(14) 2 4_545
O2 Y1 Li1 80.33(14) . 4_545
O1 Y1 Li1 40.14(12) 1_545 4_545
O1 Y1 Li1 135.52(12) 2_545 4_545
O4 Y1 Li1 39.78(12) . 4_545
O4 Y1 Li1 146.21(12) 2 4_545
Si1 Y1 Li1 55.23(4) . 4_545
Si1 Y1 Li1 130.24(5) 2 4_545
Li1 Y1 Li1 173.83(3) 3_445 4_545
F1 Y2 O3 79.85(17) 6_545 4_545
F1 Y2 O4 87.10(16) 6_545 6
O3 Y2 O4 79.08(19) 4_545 6
F1 Y2 O3 156.21(17) 6_545 .
O3 Y2 O3 80.65(12) 4_545 .
O4 Y2 O3 102.44(17) 6 .
F1 Y2 O2 80.77(17) 6_545 5
O3 Y2 O2 147.60(16) 4_545 5
O4 Y2 O2 74.23(18) 6 5
O3 Y2 O2 122.67(17) . 5
F1 Y2 O2 127.27(17) 6_545 .
O3 Y2 O2 142.17(18) 4_545 .
O4 Y2 O2 122.70(16) 6 .
O3 Y2 O2 65.36(18) . .
O2 Y2 O2 69.58(18) 5 .
F1 Y2 O1 83.46(15) 6_545 1_545
O3 Y2 O1 85.32(18) 4_545 1_545
O4 Y2 O1 162.98(18) 6 1_545
O3 Y2 O1 81.49(17) . 1_545
O2 Y2 O1 117.88(17) 5 1_545
O2 Y2 O1 74.11(16) . 1_545
F1 Y2 Si1 152.57(12) 6_545 .
O3 Y2 Si1 110.39(14) 4_545 .
O4 Y2 Si1 119.37(13) 6 .
O3 Y2 Si1 32.28(13) . .
O2 Y2 Si1 98.67(12) 5 .
O2 Y2 Si1 33.34(13) . .
O1 Y2 Si1 72.51(11) 1_545 .
F1 Y2 Y1 97.66(11) 6_545 5
O3 Y2 Y1 120.87(13) 4_545 5
O4 Y2 Y1 41.96(13) 6 5
O3 Y2 Y1 104.00(12) . 5
O2 Y2 Y1 37.66(11) 5 5
O2 Y2 Y1 84.72(11) . 5
O1 Y2 Y1 153.67(13) 1_545 5
Si1 Y2 Y1 98.19(5) . 5
F1 Y2 Y1 99.49(12) 6_545 .
O3 Y2 Y1 123.37(13) 4_545 .
O4 Y2 Y1 157.29(14) 6 .
O3 Y2 Y1 80.14(13) . .
O2 Y2 Y1 85.34(11) 5 .
O2 Y2 Y1 37.70(11) . .
O1 Y2 Y1 39.34(12) 1_545 .
Si1 Y2 Y1 53.35(5) . .
Y1 Y2 Y1 115.36(3) 5 .
F1 Y2 Li1 112.22(11) 6_545 4_545
O3 Y2 Li1 73.88(13) 4_545 4_545
O4 Y2 Li1 142.80(14) 6 4_545
O3 Y2 Li1 48.60(12) . 4_545
O2 Y2 Li1 137.97(11) 5 4_545
O2 Y2 Li1 71.33(12) . 4_545
O1 Y2 Li1 34.04(12) 1_545 4_545
Si1 Y2 Li1 51.31(4) . 4_545
Y1 Y2 Li1 149.13(3) 5 4_545
Y1 Y2 Li1 53.80(3) . 4_545
F1 Y2 Li1 115.14(11) 6_545 .
O3 Y2 Li1 74.22(12) 4_545 .
O4 Y2 Li1 30.49(13) 6 .
O3 Y2 Li1 71.95(12) . .
O2 Y2 Li1 91.06(11) 5 .
O2 Y2 Li1 108.18(11) . .
O1 Y2 Li1 148.56(13) 1_545 .
Si1 Y2 Li1 92.27(5) . .
Y1 Y2 Li1 53.40(3) 5 .
Y1 Y2 Li1 144.14(2) . .
Li1 Y2 Li1 115.53(3) 4_545 .
O1 Si1 O3 114.5(3) . .
O1 Si1 O4 116.3(3) . .
O3 Si1 O4 110.6(3) . .
O1 Si1 O2 110.5(3) . .
O3 Si1 O2 101.9(3) . .
O4 Si1 O2 101.3(3) . .
O1 Si1 Li1 145.0(2) . 4_545
O3 Si1 Li1 66.98(18) . 4_545
O2 Si1 Li1 102.78(18) . 4_545
O1 Si1 Y2 133.33(19) . .
O3 Si1 Y2 49.36(18) . .
O4 Si1 Y2 110.09(19) . .
O2 Si1 Y2 53.05(17) . .
Li1 Si1 Y2 76.12(5) 4_545 .
O1 Si1 Y1 131.2(2) . .
O3 Si1 Y1 112.98(19) . .
O4 Si1 Y1 53.8(2) . .
O2 Si1 Y1 47.61(16) . .
Li1 Si1 Y1 67.05(5) 4_545 .
Y2 Si1 Y1 74.17(5) . .
O3 Si1 Li1 101.52(19) . 4
O4 Si1 Li1 90.11(19) . 4
O2 Si1 Li1 148.26(19) . 4
Li1 Si1 Li1 105.93(7) 4_545 4
Y2 Si1 Li1 148.45(8) . 4
Y1 Si1 Li1 136.39(7) . 4
Y1 F1 Y2 138.8(2) . 6_546
Si1 O1 Li1 112.3(3) . 4
Si1 O1 Y1 121.7(3) . 1_565
Li1 O1 Y1 95.08(17) 4 1_565
Si1 O1 Y2 118.7(2) . 1_565
Li1 O1 Y2 106.4(2) 4 1_565
Y1 O1 Y2 99.30(18) 1_565 1_565
Si1 O2 Y1 100.0(2) . .
Si1 O2 Y2 141.3(3) . 5
Y1 O2 Y2 103.8(2) . 5
Si1 O2 Y2 93.6(2) . .
Y1 O2 Y2 102.11(18) . .
Y2 O2 Y2 110.42(18) 5 .
Si1 O3 Y2 124.9(3) . 4
Si1 O3 Y2 98.4(2) . .
Y2 O3 Y2 134.6(2) 4 .
Si1 O4 Li1 103.3(3) . 4_545
Si1 O4 Y2 137.0(3) . 6_556
Li1 O4 Y2 116.5(2) 4_545 6_556
Si1 O4 Y1 94.0(2) . .
Li1 O4 Y1 92.33(18) 4_545 .
Y2 O4 Y1 99.7(2) 6_556 .
O4 Li1 O4 180.0(4) 6 4
O4 Li1 O1 92.74(19) 6 4_545
O4 Li1 O1 87.26(19) 4 4_545
O4 Li1 O1 87.26(19) 6 6_565
O4 Li1 O1 92.74(19) 4 6_565
O1 Li1 O1 180.0(3) 4_545 6_565
O4 Li1 Si1 32.39(13) 6 6
O4 Li1 Si1 147.61(13) 4 6
O1 Li1 Si1 102.49(13) 4_545 6
O1 Li1 Si1 77.51(13) 6_565 6
O4 Li1 Si1 147.61(13) 6 4
O4 Li1 Si1 32.39(13) 4 4
O1 Li1 Si1 77.51(13) 4_545 4
O1 Li1 Si1 102.49(13) 6_565 4
Si1 Li1 Si1 180.00(10) 6 4
O4 Li1 Si1 67.62(15) 6 4_545
O4 Li1 Si1 112.38(15) 4 4_545
O1 Li1 Si1 28.48(13) 4_545 4_545
O1 Li1 Si1 151.52(13) 6_565 4_545
Si1 Li1 Si1 74.07(7) 6 4_545
Si1 Li1 Si1 105.93(7) 4 4_545
O4 Li1 Si1 112.38(15) 6 6_565
O4 Li1 Si1 67.62(15) 4 6_565
O1 Li1 Si1 151.52(13) 4_545 6_565
O1 Li1 Si1 28.48(13) 6_565 6_565
Si1 Li1 Si1 105.93(7) 6 6_565
Si1 Li1 Si1 74.07(7) 4 6_565
Si1 Li1 Si1 180.00(10) 4_545 6_565
O4 Li1 Y1 132.12(14) 6 3
O4 Li1 Y1 47.88(14) 4 3
O1 Li1 Y1 44.78(13) 4_545 3
O1 Li1 Y1 135.22(13) 6_565 3
Si1 Li1 Y1 122.28(5) 6 3
Si1 Li1 Y1 57.72(5) 4 3
Si1 Li1 Y1 65.17(5) 4_545 3
Si1 Li1 Y1 114.83(5) 6_565 3
O4 Li1 Y1 47.88(14) 6 5
O4 Li1 Y1 132.12(14) 4 5
O1 Li1 Y1 135.22(13) 4_545 5
O1 Li1 Y1 44.78(13) 6_565 5
Si1 Li1 Y1 57.72(5) 6 5
Si1 Li1 Y1 122.28(5) 4 5
Si1 Li1 Y1 114.83(5) 4_545 5
Si1 Li1 Y1 65.17(5) 6_565 5
Y1 Li1 Y1 180.0 3 5
O4 Li1 Y2 100.96(13) 6 4
O4 Li1 Y2 79.04(13) 4 4
O1 Li1 Y2 39.61(12) 4_545 4
O1 Li1 Y2 140.39(12) 6_565 4
Si1 Li1 Y2 127.43(4) 6 4
Si1 Li1 Y2 52.57(4) 4 4
Si1 Li1 Y2 61.55(4) 4_545 4
Si1 Li1 Y2 118.45(4) 6_565 4
Y1 Li1 Y2 62.67(4) 3 4
Y1 Li1 Y2 117.33(4) 5 4
O4 Li1 Y2 79.04(13) 6 6
O4 Li1 Y2 100.96(13) 4 6
O1 Li1 Y2 140.39(12) 4_545 6
O1 Li1 Y2 39.61(12) 6_565 6
Si1 Li1 Y2 52.57(4) 6 6
Si1 Li1 Y2 127.43(4) 4 6
Si1 Li1 Y2 118.45(4) 4_545 6
Si1 Li1 Y2 61.55(4) 6_565 6
Y1 Li1 Y2 117.33(4) 3 6
Y1 Li1 Y2 62.67(4) 5 6
Y2 Li1 Y2 180.0 4 6
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Y1 F1 2.219(4) 2
Y1 F1 2.219(4) .
Y1 O2 2.292(4) 2
Y1 O2 2.292(4) .
Y1 O1 2.354(5) 1_545
Y1 O1 2.354(5) 2_545
Y1 O4 2.471(5) .
Y1 O4 2.471(5) 2
Y1 Si1 3.056(2) .
Y1 Si1 3.056(2) 2
Y2 F1 2.219(4) 6_545
Y2 O3 2.263(5) 4_545
Y2 O4 2.291(5) 6
Y2 O3 2.317(5) .
Y2 O2 2.338(5) 5
Y2 O2 2.419(5) .
Y2 O1 2.453(4) 1_545
Y2 Si1 3.021(2) .
Si1 O1 1.624(5) .
Si1 O3 1.630(5) .
Si1 O4 1.634(5) .
Si1 O2 1.664(6) .
Si1 Li1 2.969(2) 4_545
Si1 Li1 3.151(2) 4
F1 Y2 2.219(4) 6_546
O1 Li1 2.154(5) 4
O1 Y1 2.354(5) 1_565
O1 Y2 2.453(4) 1_565
O2 Y2 2.338(5) 5
O3 Y2 2.263(5) 4
O4 Li1 2.132(5) 4_545
O4 Y2 2.291(5) 6_556
Li1 O4 2.132(5) 6
Li1 O4 2.132(5) 4
Li1 O1 2.154(5) 4_545
Li1 O1 2.154(5) 6_565
Li1 Si1 2.969(2) 6
Li1 Si1 2.969(2) 4
Li1 Si1 3.151(2) 4_545
Li1 Si1 3.151(2) 6_565
